Langmuir 2005, 21, 487-497
Simulation of Interaction Forces between Nanoparticles in the Presence of Lennard-Jones Polymers: Freely Adsorbing Homopolymer Modifiers Krishna Tej Marla and J. Carson Meredith* School of Chemical and Biomolecular Engineering, Georgia Institute of Technology, Atlanta, Georgia 30332-0100 Received July 2, 2004. In Final Form: October 11, 2004 The force between two nanoscale colloidal particles dispersed in a solution of freely adsorbing LennardJones homopolymer modifiers is calculated using the expanded grand canonical Monte Carlo simulation method. We investigate the effect of polymer chain length (N), nanoparticle diameter (σc), and colloidpolymer interaction energy (cp) on polymer adsorption (Γ) and polymer-induced forces (FP(r)) between nanoparticles in the full thermodynamic equilibrium condition. There is a strong correlation between polymer adsorption and the polymer-mediated nanoparticle forces. When the polymer adsorption is weak, as in the case of smaller diameters and short polymer chain lengths (σc ) 5, N ) 10), the polymers do not have any significant effect on the bare nanoparticle interactions. The adsorbed amount increases with increasing particle diameter, polymer chain length, and colloid-polymer interaction energy. In general, for strong polymer-particle adsorption the polymer-governed force profiles between nanoparticles show short-range repulsion and long-ranged attraction, suggesting that homopolymers would not be ideal for achieving stabilization in nanoparticle dispersions. The attraction is likely due to bridging, as well as polymer segment-segment interactions. The location and magnitude of attractive minimum in the force profile can be controlled by varying N and cp. The results show partial agreement and some marked differences with previous theoretical and experimental studies of forces in the limit of flat walls in an adsorbing polymer solution. The difference could be attributed to incorporation of long-ranged colloidpolymer potential in our simulations and the influence of the curvature of the nanoparticles.
1. Introduction Understanding and manipulating the forces governing nanoscale colloidal phenomena is the key to controlling the phase behavior and stability of nanocolloidal dispersions. Current and potential applications of nanoparticle dispersions range from additives and catalysts to controlled drug-delivery agents and biosensing quantum dots. In addition, the thermodynamically driven autonomous organization of nanoparticles into well-defined superstructures is a promising “bottom-up” fabrication approach to the development of microelectronic, optoelectronic, and photonic devices. A common way to achieve control over nanoparticle interactions is to use polymeric surface modifiers which mask out the van der Waals (VDW) forces between the particles. Examples of the use of polymeric surface modifiers in nanoparticle synthesis and dispersions include preparation of colloidal gold nanoparticles using a helical backbone polymer, poly(N,N-dihexylcarbodiimide),1 nanocomposites that include metallic particles with an organic shell of polymer (i.e., polystyrene, poly(dimethylsiloxane), poly(ethyleneoxide), poly(carbodiimides), poly(vinylpyridine), etc.)2-7 suitable for hierarchical * Author to whom correspondence should be addressed. E-mail: [email protected]
(1) Liu, Y.; Cheng, S. Z. D.; Xing, W.; Jun, H. Langmuir 2002, 18, 10500-10502. (2) Jordan, R.; Ulman, A.; Kang, J. F.; Rafailovich, M. H.; Sokolov, J. J. Am. Chem. Soc. 1999, 121, 1016-1022. (3) Beecroft, L. L.; Ober, C. K. Chem. Mater. 1997, 9, 1302-1317. (4) Corbierre, M. K.; Cameron, N. S.; Sutton, M.; Mochrie, S. G. J.; Lurio, L. B.; Ruehm, A.; Lennox, R. B. J. Am. Chem. Soc. 2001, 123, 10411-10412. (5) Fan, X.; Xia, C.; Fulghum, T.; Park, M.-K.; Locklin, J.; Advincula, R. C. Langmuir 2003, 19, 916-923. (6) Hashimoto, T.; Harada, M.; Sakamoto, N. Macromolecules 1999, 32, 6867-6870.
self-organization into nanoassemblies,8,9 and polymersilica nanocomposites that mimic natural organicinorganic materials.10,11 The ability to rationally and predictively design polymeric modifiers that would allow precise control over nanoparticle interactions is an important step toward harnessing the potential applications of colloidal nanoparticles. However, the exact nature and magnitude (relative and absolute) of the polymermediated forces between these nanoparticles are not very well understood. In addition, experimental determination of polymer-induced nanoparticle forces still remains a challenging task. What is needed is a fundamental understanding of the effects of various molecular parameters such as the nanoparticle size, polymer molecular weight and concentration, and adsorption energy on polymer adsorption and, consequently, effective interaction forces in these nanoparticle-polymer systems. This would enable us to develop molecular thermodynamic models of these systems which are a precursor to rational predictive strategies for nanoscale structural material synthesis. Homopolymer adsorption on surfaces and their resultant interactions have been studied extensively using theoretical, experimental, and computer simulation approaches as a method of achieving stabilization (as well as flocculation) in macroscopic colloidal particulate systems. For homopolymer adsorption, it is important to (7) Hicks, J. F.; Young, S.-S.; Murray, R. W. Langmuir 2002, 18, 2288-2294. (8) Fox, M. A. Acc. Chem. Res. 1999, 32, 201-207. (9) Whitesell, J. K.; Chang, H. K.; Fox, M. A.; Galoppini, E.; Watkins, D. M.; Fox, H.; Hong, B. Pure Appl. Chem. 1996, 68, 1469-1474. (10) Lu, Y.; Tang, Y.; Sellinger, A.; Lu, M.; Huang, J.; Fan, H.; Haddad, R.; Lopez, G.; Burns, A.; Sasaki, D. Y.; Shelnutt, J.; Brinker, C. J. Nature 2001, 410. (11) Sellinger, A.; Weiss, P. M.; Nguyen, A.; Lu, Y.; Assink, R. A.; Gong, W.; Brinker, C. J. Nature 1998, 394, 256-260.
10.1021/la0483461 CCC: $30.25 © 2005 American Chemical Society Published on Web 12/04/2004
Langmuir, Vol. 21, No. 1, 2005
distinguish between full thermodynamic equilibrium, wherein the chains can leave the gap between the surfaces (being in equilibrium with the surrounding bulk polymer solution), and restricted equilibrium, where the polymers between the particles are “trapped” kinetically. Experiments that measure the forces between polymer-coated surfaces utilizing the surface force apparatus (SFA)12 or an atomic force microscope (AFM)13-17 are usually carried out under some form of restricted equilibrium.18 Theoretical approaches to modeling these systems can be broadly divided into two categories. One is the self-consistent mean field (SCF) formalism which was first applied to polymer adsorption on surfaces by Scheutjens and Fleer19 and was later used to calculate free energy of interaction of two surfaces coated with polymers.20 The SCF method solves for the average equilibrium conformation adopted by a polymer under the influence of the potential imposed by the mean field of the surrounding molecules and the surface. The other approach is based on the density functional theory (DFT) models proposed by de Gennes21,22 and later developed by Pincus and co-workers.23,24 In this approach, the free energy of the system is expressed as an integral of a function consisting of a sum of the free energy of a hypothetical system which is homogeneous at the local density of the polymer segments and a term accounting for the variation in the local density, arising from the inhomogeneity of the interfacial profile. The idea here is to calculate the segment density profile that minimizes the integral free energy of the system. Both these approaches have predicted successfully the adsorbed amounts, segment density profiles, and force profile between two surfaces in the presence of adsorbing polymers. Theoretical studies based on the abovedescribed methods suggest that, at full equilibrium, there exists a monotonic attraction between the two polymercoated surfaces at all separations. At restricted equilibrium, the SCF-based theories predict that the interaction force is attractive at large distances and repulsive at short distances.20 The attraction is primarily due to bridging and, in the case of poor solvents, is in part due to polymer intersegmental attraction. However, results from the DFT approach suggest that restricted equilibrium would give rise to only monotonic repulsion under good solvent conditions.21 Both these contrasting results have also been observed experimentally.18 Monte Carlo (MC) and molecular dynamics (MD) simulation methods have also been used previously to study alkane25 and polymer solvation forces between flat walls in the limit of “gaslike” as well as “liquidlike” polymer densities.26 Depending on factors (12) Israelachvili, J. N. Intermolecular & Surface Forces, 2nd ed.; Academic Press: San Diego, 1991. (13) Goodman, D.; Kizhakkedathu, J. N.; Brooks, D. E. Langmuir 2004, 20, 2333-2340. (14) O’Shea, S. J.; Welland, M. E.; Rayment, T. Langmuir 1993, 9, 1826-1835. (15) Yamamoto, S.; Tsujii, Y.; Fukuda, T. Macromolecules 2000, 33, 5995-5998. (16) Yamamoto, S.; Ejaz, M.; Tsujii, Y.; Fukuda, T. Macromolecules 2000, 33, 5608-5612. (17) Adler, J. J.; Singh, P. K.; Patist, A.; Rabinovich, Y. I.; Shah, D. O.; Moudgil, B. M. Langmuir 2000, 16, 7255-7262. (18) Patel, S. S.; Tirrell, M. Annu. Rev. Phys. Chem. 1989, 40, 597635. (19) Scheutjens, J. M. H. M.; Fleer, G. J. J. Phys. Chem. 1979, 83, 1619-1635. (20) Scheutjens, J. M. H. M.; Fleer, G. J. Macromolecules 1985, 18, 1882-1900. (21) de Gennes, P.-G. Macromolecules 1981, 14, 1637-1644. (22) de Gennes, P.-G. Macromolecules 1982, 15, 492-500. (23) Klein, J.; Pincus, P. Macromolecules 1982, 15, 1129-1135. (24) Ingersent, K.; Klein, J.; Pincus, P. Macromolecules 1986, 19, 1374-1381. (25) Dijkstra, M. Thin Solid Films 1998, 330, 14-20. (26) Yethiraj, A.; Hall, C. K. Macromolecules 1990, 23, 1865-1872.
Marla and Meredith
such as intermolecular interactions, wall-polymer interactions, and polymer segment densities, these solvation forces have been reported to be repulsive, attractive, or oscillatory at short separations. Experimental and theoretical studies invariably involve flat and macroscopic surfaces and high-molecular-weight (long-chain) polymers. The results in the flat-wall limit can be extended to large spherical surfaces using the Derjaguin approximation, which relates the force profile between two curved surfaces to the interaction free energy between two planar surfaces. However, in the case of nanoparticles, the curvature effects become important and the Derjaguin approximation is no longer expected to hold. In addition, the mean size of the polymer chains (i.e., their radius of gyration, Rg) used for surface modification in these nanoparticle systems is comparable to the diameter of the particles (and hence would be of relatively low molecular mass). These factors make it important to ask how the polymers change nanocolloidal phenomena, in contrast to larger colloid size ranges. There have been a few recent studies that calculate the solvation forces between two nanoparticles in LennardJones (LJ) and soft-sphere fluids using MD simulations. Namely, Shinto et al.27 varied the fluid-nanoparticle interactions to study the van der Waals and solvation forces between solvophobic and solvophilic nanoparticles. Qin and Fichthorn28 also performed similar studies in which they represented the nanoparticles as rigidly fixed clusters of LJ atoms and determined the effect of particle size, shape, and roughness on the solvation forces. The force profiles obtained in both these studies are similar in form to those predicted for fluids confined between flat and infinite surfaces (attractive for solvophobic and oscillatory for solvophilic nanoparticles). However, to the best of our knowledge, there have been no reported simulation studies of interaction forces between nanoscale colloidal particles in the presence of freely adsorbing homopolymer modifiers. In this study, we calculate the polymer-mediated interaction force profiles between spherical nanoparticles in the true thermodynamic equilibrium condition using the expanded grand canonical MC method. The LJ homopolymer is used to model freely adsorbing modifiers, as it incorporates both attraction and adsorption effects. We investigate the effect of nanoparticle diameter, polymer chain length, and the polymer-particle adsorption energy on the force profiles. In addition, we also determine polymer adsorption on the particle surface, as well as the nature and orientations of the adsorbed layers, and use these results to interpret the force-distance curves. On the basis of the correlation between polymer adsorption and the force profiles, we propose the dominant mechanism which leads to attraction or repulsion in these systems. These simulations lend important insights into the physics of attractive polymer-nanoparticle mixtures, which are currently unavailable from experimental or theoretical approaches. The objective of this work is to characterize the dependence of polymer adsorption and nanoparticle interactions on the various physical molecular parameters toward the development of rational design criteria for polymer modifiers. The rest of this paper is organized as follows. In Section 2, we describe briefly the simulation details and methodology of force calculations. The effect of the various molecular parameters on adsorption of homopolymers on nanoparticles is presented in Section 3 followed by detailed results and discussion (27) Shinto, H.; Miyahara, M.; Higashitani, K. J. Colloid Interface Sci. 1999, 209, 79-85. (28) Qin, Y.; Fichthorn, K. A. J. Chem. Phys. 2003, 119, 9745-9754.
Simulation of Interaction Forces between Nanoparticles
Langmuir, Vol. 21, No. 1, 2005 489
of the polymer-mediated force profiles. We also present a comparison of our results with those obtained for macroscopic colloids in the flat-wall limit. Finally, we present some concluding remarks in Section 4. 2. Simulation Method In this work, we have simulated the net binary interaction force between colloidal nanoparticles in the presence of freely (reversibly) adsorbing homopolymer surface modifiers. The polymeric modifiers are modeled as fully flexible LJ chains in continuum. The bond length between adjacent segments in a polymer chain is maintained constant at σp. The nonbonded polymer segments interact via the cut and shifted LJ potential shown in eq 1,
[( ) ( ) ( ) ( ) ] σij rij
r e rc r > rc
where σij ) (σi + σj)/2 is the size parameter and ij is the LJ interaction energy parameter. The cutoff distance (rc) has been set to rc ) 2.5σp, and the potential has been shifted to ensure continuity at cutoff. The system consists of two spherical colloidal nanoparticles dispersed in a dilute polymer (or oligomer) solution. Three types of interactions are considered; segment-segment for nonbonded polymer sites and colloid-segment and colloidcolloid. The colloid-segment and the colloid-colloid interactions are modeled using the full LJ potential without any cutoff. The simulation variables are reduced in the standard manner, i.e., temperature T* ) TkB/pp, density F/p ) Fpσ3p, where pp is the polymer segment-segment interaction parameter, kB is the Boltzmann constant, and Fp is the bulk polymer segment density. The polymer segment density is defined as Fp ) Nnp/V, where N is the polymer chain length, np is the number of chains, and V is the volume of the simulation box. All the simulations were performed at a constant reduced temperature of T* ) 3.0, which mimics the good solvent condition for the polymer chains. In addition, this temperature is above the upper critical solution ‘theta’ temperature (UCST) of LJ polymer chains, known from previous simulations to be 2.5,29 thereby eliminating any effects of polymer phase transitions. In our simulations, the solvent is not included explicitly and the energetic effects of solvent could be modeled by changing the reduced temperature or the colloidpolymer interaction energy parameter (cp). To equilibrate polymeric modifiers between the bulk phase and the colloidpolymer (CP) region, simulations were performed in a grand canonical ensemble with N, µp, V, and T* constant, where µp is the polymer chemical potential. Figure 1 gives the schematic of the bulk polymer (Figure 1a) and the colloid-polymer (Figure 1b) simulation boxes. The dimensions of the simulation box are 40σp, in the x and y directions and 50σp, in the z direction. These box dimensions ensure that there are no artificial interactions between periodic images. Standard periodic boundary conditions apply in all directions. All the simulations were performed at a bulk polymer segment density of F/p ) 0.05. The polymermediated nanoparticle interaction forces were calculated for two different particle diameters, σc ) 10σp and 5σp. The effect of homopolymer molecular weight (i.e., chain length) was also studied by considering chain lengths of N ) 10 and 30. In addition, the effect of the strength of nanoparticle-polymer interactions (cp) on the force distance profiles was explored by varying cp from 5pp (strong attraction) to completely turning off the colloidpolymer attraction and having only a soft-repulsive interaction (obtained by using only the repulsive term in the LJ potential). pp is maintained constant at pp ) 1 in this study unless specified otherwise. Expanded Grand Canonical Ensemble Simulations. The equilibrium partitioning of polymer chains between the bulk phase and the colloid-polymer region was simulated using the grand canonical (µVT) ensemble. At the bulk densities and polymer chains lengths that we consider, the trial insertions and (29) Luna-Ba´rcenas, G.; Meredith, J. C.; Gromov, D. G.; Sanchez, I. C.; de Pablo, J. J.; Johnston, K. P. J. Chem. Phys. 1997, 107, 1-11.
Figure 1. Configuration snapshot of the bulk polymer (Figure 1a) and the colloid-polymer (Figure 1b) simulation boxes. The bulk polymer segment density is F/p ) 0.05. The snapshot of the colloid-polymer simulation box is shown for the case of σc ) 10σp, N ) 30, cp ) 1, and colloid surface-to-surface separation distance of D ) 5. deletions of the polymer molecules can be carried out very efficiently in the grand canonical ensemble by combining it with the expanded ensemble method for calculating polymer chemical potentials.30 The detailed derivation of the expanded ensemble for the calculation of chemical potentials31 and phase equilibria30 of polymer systems can be found in the literature. In addition, the details of the expanded grand canonical MC method applied to the simulation of homopolymer adsorption on two impenetrable flat surfaces are described in ref 32. Here, we adopt a similar methodology for simulation of homopolymers adsorbing on spherical nanoscale colloidal particles. Computational Method. NVT simulations of the bulk polymer solutions were first performed to generate chain chemical potentials at a given temperature (T*) and bulk polymer density (30) Escobedo, F.; de Pablo, J. J. J. Chem. Phys. 1996, 105, 43914394. (31) Escobedo, F.; de Pablo, J. J. J. Chem. Phys. 1995, 103, 27032710. (32) Meredith, J. C.; Johnston, K. P. Langmuir 1999, 15, 80378044.
Langmuir, Vol. 21, No. 1, 2005
Marla and Meredith
Table 1. Simulation Conditions Explored in This Studya case no.
1 2 3 4 5 6 7 8 9 10 11
5 5 5 10 10 10 10 10 10 10 10
10 1.0 1.0 1.067 30 1.0 1.0 3.840 30 2.0 1.0 3.840 10 1.0 1.0 1.067 20 1.0 1.0 2.457 30 1.0 1.0 3.840 30 2.0 1.0 3.840 30 5.0 1.0 3.840 30 repb 1.0 3.840 30 0.5 0.5 7.469 30 1.0 repb 14.392
/ Fp,interface Rg,bulk REED,bulk
0.0516 0.0564 0.0663 0.0603 0.0758 0.0886 0.1125 0.1522 0.0468 0.0616 0.0532
1.55 2.95 2.95 1.55 2.34 2.95 2.95 2.95 2.95 3.21 3.59
3.82 7.29 7.29 3.82 5.80 7.29 7.29 7.29 7.29 7.95 9.18
a µ is the set point chain chemical potential obtained from bulk p / is the equilibrium polymer segment simulations, and Fp,interface density in the colloid-polymer simulation box. Rg,bulk and REED,bulk are the radius of gyration and end-to-end distance of the polymer chains in the bulk. b “rep” indicates a purely repulsive interaction obtained by using only the repulsive term in the LJ 6-12 potential.
(F/p ) 0.05). The chain chemical potential was calculated by using the expanded variable-length chain ensemble.31 The accuracy of the expanded ensemble code was verified by comparing our chemical potentials to those of previous workers for hard-sphere chains.31 The nanoparticle-polymer phase was simulated using the expanded grand canonical ensemble by taking the chain chemical potential values from the bulk simulations as set points. For each simulation, the two nanoparticles (A and B) were fixed along the z axis at a specified distance from each other. The polymer chains were then added to the simulation box, and the system was allowed to equilibrate until the set point chemical potential was attained. Thermal equilibrium in the simulation box was achieved by performing chain displacements using the continuum configurational bias (CCB) algorithm,33-35 in which a section of the chain is cut and regrown into low-energy conformations after scouting Nsp trial positions. Nsp was set to 6 in our simulations. Then, the forces due to the polymer chains on each nanoparticle (FAP(r) and FBP(r)) were calculated. This ensured that the force at each distance was calculated at “true” thermodynamic equilibrium. Further, the chain end-to-end distance, orientation with respect to the nanoparticle, and segment density profiles were also calculated. Individual simulations were performed at many distances to obtain the forcedistance profile. The forces were calculated from the nearest center-to-center separation (rc-c) between the nanoparticles of rc-c ) σc + 1σp in increments of 1σp up until approximately rc-c ) 2.5 σc. The forces reported in this paper were normalized by subtracting the force at “infinite” separation, where the nanoparticle surfaces were far enough not to affect one another significantly. The expanded grand canonical ensemble code was verified by comparing average chemical potentials, densities, and chain conformational properties to results from NVT simulations. In most cases, (20-40) × 106 equilibrium steps and (120-180) × 106 averaging steps were required at each separation distance to obtain statistically significant averaged values of the properties of interest. In this work, one MC step corresponds to one attempted move. The statistical error in the forces was based on the statistical inefficiency parameter.36 Note that all error bars have been omitted from the figures unless they were larger than the symbols representing the data points. The details of the all the cases and conditions that were explored in this study are given in Table 1, where µp is the set chain chemical potential obtained from bulk polymer simulations, Rg,bulk and REED,bulk are the polymer radius of gyration and end-to-end distance, respec/ is the equilibrium tively, in the bulk region, and Fp,interface average polymer segment density in the nanocolloid-polymer simulation box (also referred to as the interface region or colloidpolymer region in this paper). (33) de Pablo, J. J.; Laso, M.; Suter, U. W.; Cochran, H. D. Fluid Phase Equilib. 1993, 83, 323-331. (34) Mooij, G. C. A. M.; Frenkel, D. Mol. Phys. 1991, 74, 41-47. (35) Siepmann, J. I. Mol. Phys. 1990, 70, 1145-1158. (36) Allen, M. P.; Tildesley, D. J. Computer Simulation of Liquids; Clarendon Press: Oxford, 1987.
Force Calculations. The total polymer-mediated interaction force between the colloidal nanoparticles is the sum of the direct nanoparticle-nanoparticle force (FD) and the forces acting on the nanoparticles due to the adsorbing polymers (FP). The direct interaction force between the uncoated nanoparticles FD(r) is obtained by analytical integration of eq 1.
∂Ucc(r) 48 σc FD(r) ) ) ∂r r r
The forces on nanoparticles A and B due only to the polymer chains, FAP(r) and FBP(r), are calculated by using a virial relation that must be ensemble-averaged over many polymer configurations, i)Nnp
where ucp is the colloid-polymer LJ segment interaction potential. The net polymer contribution to the nanoparticle interaction is calculated from the individual nanoparticle-polymer forces using27,28
1 FP(r) ) 〈rˆ AB ‚ (FAP - FBP)〉r 2
rˆ AB ) (rA - rB)/|rA - rB|
where rˆ AB is a unit vector pointing from particle B to particle A. In our simulations, the nanoparticles are fixed along the z axis (zA > zB), and hence, due to symmetry in the (x,y) plane, only the z component of force contributes. The total binary nanoparticle interaction force, FTOT(r), is given by FTOT(r) ) FP(r) + FD(r). It must be noted here that the use of the LJ pair interaction potential to model the interaction between the colloid and polymer segments is, at best, a gross oversimplification of reality. However, we believe that the potential does capture the salient features of colloid (or nanoparticle)-polymer systems with primarily dispersive interactions. The homopolymer modeled here is a nonpolar organic molecule. What is missing here is an accounting for the density of the nanoparticle and an integration of the LJ potential between all the atoms in the nanoparticle and each polymer segment, in the manner of the Hamaker microscopic approach.12,37 In this case, the potential becomes much more long ranged, e.g., (σ/r)9 - (σ/r)3. However, the generic feature of the attraction magnitude increasing linearly with colloid size occurs in both the pure and integrated LJ forms. Hence, the 6-12 LJ potential, though not quantitatively exact, does approximate the physics of van der Waals interactions in these systems. It is noteworthy to consider the effect of particle diameter on the direct force profiles obtained from differentiating LJ-type power law potentials. Consider a general power-law potential of the form [(σ/r)m - (σ/r)n]. For this potential, the force, f(r), is given by
f(r) ) -
∂U 1 σ ) m ∂r r r
The minimum in the force, obtained by setting ∂f/∂r ) 0, occurs at
rmin ) σ
m(m + 1) n(n + 1)
and is given by,
fmin ) -n
m - n n(n + 1) m + 1 m(m + 1)
1 A )σ σ
For m,n > 0 and m > n, A is always greater than 0. This implies that the magnitude of fmin increases with decreasing particle (37) Henderson, D.; Duh, D.-M.; Chu, X.; Wasan, D. J. Colloid Interface Sci. 1997, 185, 265-268.
Simulation of Interaction Forces between Nanoparticles
Figure 2. Direct LJ interaction force FD(r) between the two particles versus separation distance at different particle diameters (σc). FD(r) is calculated from eq 2.
Figure 3. Polymer segment density profiles in the z direction in the nanoparticle-polymer simulation box at two particle sizes σc ) 5σp, 10σp and chain lengths N ) 10, 30. Values in plot are σc, N. cp ) pp ) 1. The plots are for a surface-to-surface separation (D) of 5σp between the particles, where D is defined as D ) rc-c - σc. The two vertical dashed lines indicate the location of the nanoparticle centers. size. This is illustrated in Figure 2 which shows the direct force profile (from eq 2) as a function of particle diameter. The plot shows that the minimum in the force profile becomes lower and moves to a closer separation distance as the nanoparticle diameter becomes smaller, making them relatively more difficult to stabilize.
3. Results and Discussion 3.1 Adsorption of Homopolymer Modifiers on the Colloidal Nanoparticles. Effect of Particle Diameter (σc)and Chain Length (N). The force-distance profile between nanoparticles dispersed in a solution of freely adsorbing homopolymers is correlated strongly with the amount of polymer adsorbed on the nanoparticles and the nature of the adsorbed layers. We first explore the dependence of adsorption on the various molecular parameters (σc, N, cp, pp) to obtain a better understanding of the physical phenomena that govern the polymer-induced nanoparticle forces. Figure 3 shows the polymer segment density profiles in the z direction at two particle sizes σc ) 5σp, 10σp and chain lengths N ) 10, 30. The plots are for a surface-to-surface separation (D) of 5σp between the particles, where D is defined as D ) rc-c - σc and rc-c is the center-to-center separation. The locations of the nanoparticle centers are represented by the dashed lines parallel to the y axis in Figure 3. At constant chain length, the local segment density near the particle is greater for
Langmuir, Vol. 21, No. 1, 2005 491
Figure 4. Effect of changing the colloid-polymer interaction energy parameter cp at σc ) 10σp, N ) 30 and pp ) 1 on the polymer segment density profiles in the z direction in the nanoparticle-polymer simulation box. The plots are for a surface-to-surface separation (D) of 5σp between the particles, where D is defined as D ) rc-c - σc. The two vertical dashed lines indicate the location of the nanoparticle centers.
larger colloids. Increasing the colloid diameter increases the range of the LJ attraction bringing more chains from the bulk under the attractive influence of the colloidal particle. In addition, the increased surface area available for particle-polymer contacts also enhances adsorption. Consequently, the amount of polymer adsorbed increases with increasing particle diameter. A measure of the attractive influence of the particle diameter is reflected / in the Fp,interface values shown in Table 1 (cases 2 and 6), / for σc ) 10σp is much higher than the where Fp,interface / values reported value for σc ) 5σp. Note that the Fp,interface in Table 1 are averaged over all separations (D) for each specific case. Figure 3 also shows that for constant σc, the increase in polymer segment density in the colloidpolymer region is greater for longer chains. This is because the entropy loss associated with chain adsorption is lower for longer chains The adsorption of these LJ homopolymers on single LJ nanoparticles was discussed in detail in a recent publication.38 The nature of adsorption is dependent on the ratio of polymer to particle size. When Rg . σc, the particle only interacts locally with a few polymer segments and adsorption is linearly dependent on N. For Rg , σc, adsorption is independent of N and nearly all segments in the chain interact with the particle. In this regime, chain conformations are modified considerably relative to bulk dimensions, e.g., the chains flatten at the particle interface. The ratio of Rg components parallel-versusperpendicular to the surface varies between 2 and 3.38 In this paper, 0.155 < Rg/σc < 0.49, which does not correspond with either of the extreme limits above. In fact, most cases we explore here cover Rg/σc values of 0.3-0.49 (specifically the σc ) 10 cases), where adsorption is represented by a power-law dependence on N, Γ ∼ Np, with p < 0.5. Only the Rg/σc ) 0.155 (σc ) 5) case approaches the smallparticle limit, in which the adsorption was quite weak. Effect of Colloid-Polymer Interaction Energy (cp). Figure 4 shows the effect of changing the colloid-polymer interaction energy parameter, cp, at σc ) 10σp, N ) 30, D ) 5σp, and pp ) 1 on the segment density profiles. Varying this parameter allows us to understand the effect of tuning the solvent quality of the polymer. When cp is increased compared to pp, the polymer has a greater affinity for the particle surface than the polymer solution, and this in (38) Marla, K. T.; Meredith, J. C. Langmuir 2004, 20, 1501-1510.
Langmuir, Vol. 21, No. 1, 2005
Marla and Meredith
Figure 5. Effect of changing the polymer-polymer interaction energy parameter pp at σc ) 10σp, N ) 30 and cp ) 1 on the polymer segment density profiles in the z direction in the nanoparticle-polymer simulation box. The plots are for a surface-to-surface separation (D) of 5σp between the particles, where D is defined as D ) rc-c - σc. The two vertical dashed lines indicate the location of the nanoparticle centers.
turn results in increased polymer adsorption. Figure 4 also shows the effect of turning off the colloid-polymer attraction wherein only the repulsive part of the LJ 6-12 potential is used to model the colloid-polymer interactions. This is equivalent to the case of suspending nanoparticles in a solution of nonadsorbing polymer solution, and as expected, there is a depletion of polymer segment density in the vicinity of the nanoparticles. The solvent quality could also be tuned by varying pp while holding cp constant. Figure 5 shows how the polymer segment density profiles are influenced by changing pp, at σc ) 10σp, N ) 30, D ) 5σp, and cp ) 1. In general, as pp is varied from being purely repulsive (hard-sphere chains) to pp ) 1, there is an increase in the polymer segment density in the CP region. As pp is decreased compared to cp, one would expect that the polymer segment density near the particle would progressively increase, which is not the case in Figure 5. Although the polymers have a comparatively stronger affinity for the particle surface (when pp is decreased compared to cp), the decreased polymer segment-segment interaction limits the number of chains that can be adsorbed. At pp ) 1.5 (plots not shown), we found that the density of / ) polymer in the CP region oscillated between Fp,interface 0.026 and 0.16, suggesting that we had reached a coexistence point. This case was not explored further, as phase transition effects are beyond the scope of this paper. It is interesting to compare the cases of cp ) 2, pp ) 1 (Figure 4) and cp ) 1, pp ) 0.5 (Figure 5). The ratio cp/pp ) 2 for both these cases; however, the polymer segment density in the vicinity of the colloid is almost twice in the case of cp ) 2, pp ) 1, indicating that the effect of tuning cp is significantly different from varying pp. A notable feature of all the segment distribution plots in which attraction dominates is that, as D decreases, the local polymer segment density between the planes passing through the centers of the two nanoparticles and perpendicular to the z axis increases monotonically. For polymer that can freely adsorb-desorb, it would be expected that the polymers would leave the region between the nanoparticles due to entropic considerations as D is reduced. On the other hand, the polymers in this region would also experience doubly strong enthalpic interactions due to the two particles in their close proximity, which could offset the entropic penalty and result in increased adsorption. Changes in the polymer segment density in the interface region can be examined by integrating the
Figure 6. Excess adsorbed amount per unit surface area of the particle (Γs) calculated from eq 8 vs nonoparticle surfaceto-surface separation distance (D) for the various cases explored in this study. (a) Effect of particle size and chain length at cp ) pp ) 1. Values in the plot are σc, N. (b) Effect of colloidpolymer and polymer-polymer interaction energy parameters. Values in the plot are cp, pp at σc ) 10 σp, N ) 30. “R” indicates a purely repulsive interaction.
segment density profiles to yield adsorption isotherms with,
/ / (r) - Fp,bulk (r))2πr2dr ∫σl /2/2(Fp,interface
where Γs is the excess adsorption of the polymer segments per unit surface area of the particle, σcp is defined as (σc + σp)/2, lb is the length of the simulation box, and / Fp,interface (r) is the polymer segment density in the CP region (averaged over spherical angles θ and φ) at a distance r from the center of the particle. Γs reported in this paper is averaged over both the particles in the simulation box and is reported on a per particle basis. Figure 6 shows a plot of Γs versus nanoparticle separation distance (D) for all the cases examined in this paper. The effect of particle size and chain length at cp ) pp ) 1 is shown in Figure 6a, and the effect of colloid-polymer and polymer-polymer interaction energy parameters (cp and pp) at σc ) 10σp, N ) 30 is shown in Figure 6b. In general, for all cases, Γs increases very slightly as D decreases for reasons discussed above. Also the excess adsorbed amount increases with σc, N, cp, and pp in agreement with the segment density profiles in Figures 3-5. When the colloid-polymer attraction is turned off, Γs is negative, indicating a depletion of polymer chains in the CP region (Figure 6b). The chain adsorption-desorption phenomenon is a reversible process, and a quantitative measure of this reversibility can be obtained by calculating the average longevity fraction (Ft) of the chains. Ft is defined as the fraction of chains that do not desorb from the nanoparticle after adsorption.38 Figure 7 shows a plot of Ft versus separation distance for the various cases explored in this study. For all cases, Ft seems to increase
Simulation of Interaction Forces between Nanoparticles
Langmuir, Vol. 21, No. 1, 2005 493
Figure 7. Longevity fraction (Ft) defined as the fraction of chains that do not desorb from the particle after adsorption versus separation distance (D) for the various cases explored in this study. (a) Effect of particle size and chain length at cp ) pp ) 1. Values in the plot are σc, N. (b) Effect of colloidpolymer and polymer-polymer interaction energy parameters. Values in the plot are cp, pp at σc ) 10σp, N ) 30. “R” indicates a purely repulsive interaction.
Figure 8. Force-distance plots (polymer mediated force FP(r) vs D) for diameters of σc ) 5σp (a) and 10σp (b) at different chain lengths. cp ) pp ) 1. The direct force between the nanoparticles (FD) calculated from eq 2 is also shown for comparison.
marginally with decreasing separation distance between the nanoparticles, which corroborates the argument presented above for increased adsorption as D decreases. The longevity fraction for σc ) 10σp, N ) 30 is about three times the value for σc ) 5σp, N ) 30, indicating the relatively stable nature for the adsorbed layer for σc ) 10σp (Figure 7a). In fact, for σc ) 5σp, Ft is very close to zero, resulting in an adsorbed layer where adsorptiondesorption phenomena proceed quite readily. Also, at a constant particle diameter, Ft is higher for longer chains because of the larger number of polymerparticle contacts that are formed. Although individual polymer segments desorb easily, the desorption energy required for an entire chain can be quite high and increases with chain length. Ft also increases monotonically with increasing cp and pp (Figure 7b), further supporting the trends obtained for adsorption and the segment density profiles. These insights into the adsorption phenomena on spherical nanoparticles will be used to interpret the force profiles observed below. 3.2 Polymer-Induced Interaction Forces between Nanocolloids. Effect of Nanoparticle Diameter (σc) and Chain Length (N). Figure 8 shows a plot of force due to the polymer chains (FP) between two nanoparticles for diameters of σc ) 5σp (Figure 8a) and 10σp (Figure 8b) at different chain lengths. The direct force between the nanoparticles (FD) calculated from eq 2 is also shown for comparison. In all force profiles the x coordinate is taken to be D ) (rc-c - σc). At σc ) 5σp, FP is very small compared to FD and is in fact close to zero for both polymer chain lengths N ) 10, 30, indicating that the polymers do not have a significant effect on the nanoparticle interactions. For σc ) 10σp, the force-distance profile is similar in form and comparable in magnitude to the direct nanoparticle
forces (FD). The attractive minimum in FP occurs at D ≈ 6, and then there is a repulsive maximum at D ≈ 2 for both chain lengths after which the force seems to decrease slightly (at D ≈ 1). Also, the polymer-induced attractive force is stronger and also the repulsive maximum is higher for N ) 30 as compared to N ) 10. As mentioned earlier, the effect of particle size and polymer chain length on the force profile is determined by their effect on polymer adsorption. From results of the adsorption studies, an increase in either σc or N results in increased adsorption / , which in turn effect an increase in and a higher Fp,interface the magnitude of both attraction and repulsion in the polymer-mediated force profile. Figure 9 shows equilibrated configuration snapshots of the nanoparticle-polymer simulation box for σc ) 5σp, N ) 30 (Figure 9a) and σc ) 10σp, N ) 30 (Figure 9b). The snapshots are for a separation distance of D ) 5 between the nanoparticles. For σc ) 10σp, a thick layer of adsorbed polymer is formed around the nanoparticles (shaded in dark in Figure 9) combined with a dense accumulation of polymers in the interparticle region, whereas for σc ) 5σp, there is no significant adsorbed layer and the polymers only form a low-density fluidlike field around the particle. The polymer-induced attraction between nanoparticles may be attributed to (i) bridging, (ii) depletion attraction, and (iii) interactions between the segments of adsorbed polymer chains or a combination of the above factors. (i) Bridging occurs when segments of an individual polymer chain adsorb on more than one particle surface. The conditions for bridging are a strong segment-particle attraction and accessible adsorption sites on both particle surfaces. Bridging gives rise to an entropic tension in the polymer chain, and the polymers gain conformational entropy by decreasing the separation between the particle
Langmuir, Vol. 21, No. 1, 2005
Figure 9. Equilibrated configuration snapshots of the nanoparticle-polymer simulation box for σc ) 5σp, N ) 30 (a) and σc ) 10σp, N ) 30 (b). The snapshots are for a surface-to-surface separation distance of D ) 5 between the nanoparticles. The polymer chains adsorbed on the nanoparticle surface are shaded in dark and the bulk chains are in white.
surfaces. At σc ) 5σp for both chain lengths N ) 10, 30, adsorption is low due to the small range of particlesegment attraction and the contribution of bridging is marginal. This was confirmed by monitoring snapshots of the equilibrated CP simulation box and counting the number of bridging chains. On average, there was not more than one bridging chain at separations D ≈ 6, for σc ) 5σp. When particle size is doubled, σc ) 10σp, polymer adsorbs strongly and forms a thick layer with high surface coverage that would be expected to prevent accessibility to adsorption sites on the opposite particle. However, this would be true only under restricted equilibrium conditions where the nanoparticles approach on a time scale faster than chain relaxation. Our study is performed under equilibrium conditions where adsorption-desorption of polymer is reversible at each separation distance. This leads to the possibility of bridging even under high surface coverage. For σc ) 10σp and N ) 10, the range over which the bridging attraction occurs decreases as compared to
Marla and Meredith
N ) 30, and this is partially responsible for the minor shift in the force minimum to a closer separation distance (D). The contribution of bridging to the total attraction is expected to be higher for larger particle sizes and longer chains. (ii) Depletion attraction is due to an osmotic force exerted by the polymer on the nanoparticles due to the difference in polymer concentration in the bulk and the region between the two nanoparticles. Although depletion attraction is associated primarily with nonadsorbing polymer solutions, it has been observed experimentally that short-ranged depletion attraction can occur between surfaces containing weakly adsorbed polymers.39 The physisorbed layers constitute a new surface which experiences an osmotic depletion attraction with the polymercoated surface of another particle. For σc ) 5σp, the adsorption is weak, suggesting that depletion attraction could be acting between the particles contributing to the overall attraction. In addition, the onset of attraction occurs approximately at D ) 2Rg for both polymer chain lengths, which is consistent with the theoretically expected range of 2Rg.40-42 At σc ) 10σp, the adsorption is strong and the polymer segment density between the particle surfaces is higher than on the outside. This almost precludes the possibility of any depletion attraction. Hence, it is unlikely that the depletion effect would contribute significantly to the overall attraction in this case (σc ) 10σp, N ) 10, 30). (iii) Attraction that is driven by polymer segmentsegment interactions is usually associated with the poor solvent condition, wherein polymer segments prefer contact with one another over contact with solvent, resulting in enhanced polymer adsorption on the particle surface. In our case, although the polymers are in the good solvent condition at T* ) 3.0, the adsorption is driven by the particle-polymer adsorption energy which increases with σc and N. At σc ) 10σp, as the separation distance between the particles is decreased, the polymers already adsorbed to each individual particle experience strong attractive interactions from both of the particles. The favorable energetic interactions experienced by the polymers apparently dominate the entropic loss, causing them to prefer this interparticle region. This, in turn, results in a large number of favorable polymer segmentsegment contacts, which further add to the driving force for the polymers to reside in this region. Figure 10 shows the segment density profiles in the z direction at different separation distances between the nanoparticles for σc ) 10σp and N ) 30. The plots show that the polymer segment density in the central plane of the simulation box, corresponding to the region between the two nanoparticles, increases with decreasing separation distance (D), corroborating the arguments presented above. Hence, at σc ) 10σp, it is likely that the polymer segment-segment interactions are primarily responsible for the attraction in the force profile. However, for σc ) 5σp, the lack of a dense adsorbed layer indicates that segment-segment interactions do not play a significant role in the polymerinduced forces. Short-Range Repulsive Forces. As the separation between the nanoparticles decreases to D e 3, the polymerinduced forces pass through zero and become repulsive in nature. At this separation, there is space available only for one physisorbed monolayer on each particle in the (39) Ruths, M.; Yoshizawa, H.; Fetters, L. J.; Israelachvili, J. N. Macromolecules 1996, 29, 7193-7203. (40) Asakura, S.; Oosawa, F. J. Chem. Phys. 1954, 22, 1255-1256. (41) Asakura, S.; Oosawa, F. J. Polym. Sci. 1958, 33, 183. (42) Vrij, A. Pure Appl. Chem. 1976, 48, 471-483.
Simulation of Interaction Forces between Nanoparticles
Figure 10. Polymer segment density profiles in the z direction in the nanoparticle-polymer simulation box at different nanoparticle surface-to-surface separation (D, values in legend). (σc ) 10σp, N ) 30 and cp ) pp ) 1)
Figure 11. Force-distance plots (polymer mediated force FP(r) vs D) for different values of the colloid-polymer interaction strength: - O - cp ) 1, - 0 - cp ) 2, - ) - cp ) 5, - 2 - cp ) repulsive (σc ) 10σp, N ) 30 and pp ) 1). The direct force between the nanoparticles (FD, - - -) calculated from eq 2 is also shown for comparison.
region between the particle surfaces. As these monolayers come into contact, entropic steric effects dominate to result in a repulsive force between the particles. Again, with increasing σc and N, the physisorbed monolayer would be attached more strongly to the surface, resulting in stronger repulsive forces, as indicated in the force profiles (Figure 8). Effect of Colloid-Polymer Interaction Energy (cp). To explore the hypothesis that segment-segment interactions between adsorbed polymer chains are the primary reason for polymer-induced attraction between spherical nanoparticles, we calculated the force-distance plots (shown in Figure 11) for different values of the colloidpolymer interaction strength ranging from cp ) 1pp to cp ) 5pp. The particle diameter, polymer chain length, and pp were kept constant at σc ) 10σp, N ) 30, and pp ) 1 for this study. As cp is increased from 1pp to 5pp, the magnitude of the maximum attractive force increases almost linearly with cp. However, the location of maximum attraction does not shift significantly and occurs at D ≈ 6 for all three cases. The adsorption and polymer segment density between the particles increase with cp (see Figures 4 and 6), resulting in increased attraction due to segmentsegment interactions. Although bridging contribution to the attraction is likely to increase with cp, it would still be less compared to the segment-segment interactions. To verify this, we determined the average number of bridging chains (nbridge) as a function of separation distance (D) at different values of cp and found only a marginal
Langmuir, Vol. 21, No. 1, 2005 495
Figure 12. Force-distance profiles (polymer mediated force FP(r) vs D) for pp ) 0.5, 1 and the case of soft-repulsive interactions between polymer segments (σc ) 10σp, N ) 30 and cp ) 1). The direct force between the nanoparticles (FD) calculated from eq 2 is also shown for comparison.
increase in nbridge as cp is increased from 1pp to 5pp. On / increased from 0.08 to 0.15 as cp the other hand, Fp,interface is increased from 1pp to 5pp. Also, the depletion effect is expected to become progressively insignificant as cp increases. It is also noteworthy that, as the strength of the colloid-polymer interactions increases, there are relatively more oscillations in the force profiles (e.g., see the force profile for cp ) 5pp between D ) 3 and 10). As mentioned before, the increase in polymer segment density in the region between the particles with cp results in liquidlike densities in this region and it is likely that the oscillations are due to packing effects. Previous simulations have shown that the solvation forces for LJ nanoparticles in a solvophilic liquid are oscillatory in nature due to packing and molecular structural effects.27,28 Figure 11 also shows the FP profile for the case of purely repulsive interaction between the nanoparticle and the polymers (nonadsorbing polymer). In this case, FP ≈ 0 for D > 6 and for D < 6, the force is purely attractive for all separations right until the particle surfaces come in contact with each other. These results are consistent with the phenomenon of depletion attraction which is expected to be the solely responsible for attraction in the case of nonadsorbing polymers. The onset of attraction which occurs at D ≈ 2Rg is also in agreement with theoretical predictions.40-42 The magnitude of this attraction, however, is very small compared to the adsorbing polymer case, and this further supports the argument that depletion effect (though present) does not play a significant role in the attraction mechanism for adsorbing polymers. Effect of Polymer-Polymer Interaction Energy (pp). Figure 12 shows the force-distance profiles for pp ) 0.5, 1 and the case of soft-repulsive interactions between polymer segments (σc ) 10σp, N ) 30, and cp ) 1). As pp is reduced from 1 to 0.5, the attractive minimum becomes less negative. Making the polymer-polymer interaction purely repulsive (only excluded volume interactions) has no significant effect on the force profiles. Reducing the value of pp, while holding cp constant, enables us to progressively turn off the contribution of depletion and segment-segment attraction to the polymer-induced particle-particle attraction. The condition of soft-repulsive interactions between polymer segments and cp ) 1 (attraction between polymer and particle), though not realistic, allows us to isolate polymer-induced attraction due to bridging from other mechanisms. The attraction observed in this case is due solely to bridging, and the magnitude of this attraction compared to the case of cp ) 1, pp ) 1 indicates that bridging contribution, though
Langmuir, Vol. 21, No. 1, 2005
significant, is secondary to the effect of segment-segment interaction. Comparison to Force Profiles in the Flat-Wall Limit. As mentioned earlier in the Introduction, most of the previous studies of interactions between layers of adsorbed polymer have been for the case of flat walls or macroscopic colloids. It is interesting to make a comparison between the adsorption and force profiles in the flat-wall limit to our simulation results for high-curvature nanoscale colloids. For flat walls with adsorbing homopolymer in full equilibrium, theory and simulation show an attractive polymerinduced force over the entire interaction range.20,21 A minimum in the free energy occurs when a monolayer of polymer segments lies flat between the two surfaces. The adsorbed amount passes through a weak maximum but then decreases as separation distance decreases until all the chains are “squeezed” out into the bulk.20 At full compression, the plates touch directly with no polymer adsorbed. In the case of nanoparticles with strong polymer-particle attraction (e.g., σc ) 10σp, N ) 30, cp ) pp ) 1, Figure 8b), the polymer-induced force passes through a minimum at approximately 2Rg but then becomes repulsive at about D ≈ 3, in contrast to the flat-wall case. The excess adsorption increases slightly as D decreases and passes through a maximum as in the flat-wall case. However, even in the limit of two particles touching each other, a finite amount of excess polymer remains on the curved sections of the particles just above and below the contact point. We propose that the difference in force and adsorption at close distances between flat walls versus nanoparticles is due to the influence of curvature on the structure and entropy of the polymer layers. For the same surface-to-surface distance, flat walls allow significantly less available volume (and hence less conformational entropy) compared to curved surfaces. As a result, the polymers that are in the region between the nanoparticle surfaces lose comparatively less entropy as the surfaces are compressed, while gaining favorable attractive energetic interactions from the particles, causing them to prefer this region (see Figure 10). As far as the force profiles are concerned, the pure attraction observed in the case of flat walls has been attributed primarily to bridging and depletion. Our results from the investigation of the effect of cp and pp on the force profiles suggest that, in addition to bridging, the polymer segment-segment attraction also contributes significantly to the polymer-induced attraction between the high-curvature nanoparticles. Also, the repulsion between the nanoparticles observed at short distances is likely due to the steric effects between the strongly adsorbed polymer layers that remain even at D ) 0. It is interesting to note in passing that, in the case of strong polymer-particle attraction, our simulated nanoparticle force profiles (in the full equilibrium condition) resemble qualitatively the nature of interaction profiles between flat walls with adsorbing polymers in the restricted equilibrium condition.20 Consideration of Multiple-Particle Interactions and Effects of Charge. In this work, we have considered a binary nanoparticle interaction, which is applicable to dilute suspensions. However, in more concentrated dispersions, multiple-particle interactions may also affect the polymerinduced force between two particles (e.g., the force averaged over all pairs of nanoparticles). Although we have not performed direct force measurements for concentrated dispersions, we have calculated chemical potentials in concentrated dispersions, which indicate the polymer solvation forces.43 From NVT simulation, we found that increasing colloid concentration at constant Fp results in less adsorption per particle and less polymer-
Marla and Meredith
particle contacts, which might imply a weaker polymerinduced force between the nanoparticles relative to the two-polymer case. For calculating multiparticle forces, an alternative method being explored is using grand-canonical simulation to obtain the potential of mean force (PMF) from colloid-colloid radial distribution functions. The PMF is differentiated to obtain the net binary force, from which the bare colloid-colloid force which could be subtracted to yield the polymer contribution to the net colloid-colloid forces. The model utilized here has considered only van der Waals attractions, whereas some important nanoparticle dispersions and nanocomposites utilize nanoparticles with charged surfaces. Most notable among these are the layered-silicate clays, although other examples exist.44 Surfactants used to disperse charged nanoparticles in organic solvents often have an oppositely charged headgroup and are ion-exchanged in aqueous solution to cover the particle. Once placed in an organic solvent, the surfactant would behave similar to an irreversibly grafted surfactant tail. We consider irreversibly grafted surfactants in a future publication. Due to the low dielectric constant of organic solvents, the Coulombic effects would be too weak to have a significant effect, except perhaps at very close distances. However, in water, the Coulombic effects of nanoparticle surface charge would be expected to play a much more important role in determining the colloid-colloid interaction forces, relative to the van der Waals interactions considered here. In fact, there are many examples of electrostatically stabilized dispersions of nanoparticles.44 Due to the significantly longer range of the Coulombic potential, adjustment to the periodic boundary conditions used in the simulation technique would be required before making calculations for charged systems. 4. Conclusions In this paper, we present a simulation study of interaction forces between nanoscale colloidal particles in the presence of freely adsorbing homopolymer modifiers in the full thermodynamic equilibrium condition. Using the expanded grand canonical MC simulation method, we have investigated the effect of polymer chain length, colloid diameter, and colloid-polymer interaction energy on polymer adsorption and polymer-induced force profiles between two spherical nanoparticles. The results are markedly different from those observed in the Derjaguin limit, wherein the colloidal particles are represented as flat walls. In general, we found that, at small particle diameters and short polymer chains lengths (σc ) 5σp, N ) 10), the polymers do not adsorb strongly and have no significant effect on the nanoparticle interactions. With increasing particle diameter and polymer chain length (σc ) 10σp, N ) 30), there is increased adsorption and the polymer-induced forces between the nanoparticles are comparable to the direct nanoparticle VDW forces. Specifically, the polymer-induced forces are repulsive at short separations (D < 3σp) and attractive at larger separations with the attractive minimum at D ≈ 6σp. The attractive minimum in the force is lower for longer chains and increasing colloid-polymer interaction energy (cp). The attractive forces are attributed primarily to polymer intersegmental interactions and bridging. These results provide the rationale why adsorbing homopolymers are not a good stabilizer for nanoparticle (43) Quant, C. A.; Meredith, J. C. Macromolecules 2004, submitted for publication. (44) Alexandre, M.; Dubois, P. Mater. Sci. Eng. R 2000, 28, 1-63.
Simulation of Interaction Forces between Nanoparticles
dispersions. However, it must be noted that in our simulations the bare nanoparticles are fixed initially at a specified distance and polymers are added to the system and are allowed to equilibrate, after which the force is calculated. While these force-profiles are representative of the true thermodynamic equilibrium condition, the thermodynamic minimum in free energy (corresponding to polymer-induced nanoparticle flocculation) may not necessarily be achieved in “real-world” experiments. To illustrate this point, consider a dilute nanoparticle dispersion in which the added homopolymer modifier adsorbs strongly before the nanoparticles come into contact with each other. If two particles coated with adsorbed polymer collide at Brownian velocities in solution, in addition to the kinetic thermal energy barrier, it is expected that there would be an initial repulsion between the adsorbed polymer layers which may prevent flocculation. To verify this, it would be interesting to simulate these nanoparticle-polymer systems in the restricted equilibrium limit using the canonical NVT ensemble. It is also noteworthy
Langmuir, Vol. 21, No. 1, 2005 497
that the adsorbing homopolymers shift the minimum in force profile to a larger separation distance between the nanoparticles as compared to the minimum in the bare particle-particle VDW dispersion force (which occurs at 21/6σc for the LJ potential). The location of the attractive minimum and the thermodynamic minimum (corresponding to FP ) 0) could be controlled by varying the polymer chain length, and the magnitude of the attractive minimum can be controlled by the colloid-polymer interaction energy parameter. While it is known that selfassembled superstructures of nanoparticles can be prepared as equilibrium products, the ability to control the thermodynamic and force minimum using the above parameters provides a molecular mechanism for nanoparticle self-assembly with controlled lattice spacing which could be potentially useful for photonic and optoelectronic devices. LA0483461